Silicon Quantum Dots Grown by Ion Implantation and › ... › docs ›...
Embed Size (px)
Transcript of Silicon Quantum Dots Grown by Ion Implantation and › ... › docs ›...
Silicon Quantum Dots Grown by Ion Implantation and
Submitted in fulfillment
Mid Spring 2007 Semester Presentations
University of Rochester
Rochester, New York
INTRODUCTION Since the 1960’s quantum-size effects have been observed in three dimensional
semiconductor nanocrystals. These effects have limited the motion of electrons and holes in semiconductor nanocrystals from one to three spatial directions. Nanocrystals that confine the motion of electrons/holes in one spatial direction and allow for free propagation in the other two spatial directions are called quantum wells. Quantum wires are nanocrystals that confine the motion of electrons/holes in two directions and if a nanocrystal confines the electron/holes in three directions it is called a quantum dot. These quantum size effects can be due to electrostatic potentials, the presence of an interface between different semiconductor materials, the presence of the semiconductor surface or due to a combination of these. In the case of a semiconductor nanocrystal, the quantum size effects are due to the crystalline properties of the semiconductor surface. Semiconductor nanocrystals that confine the electron/holes in three directions and are smaller then 10nm are referred to as a quantum dots. These structures are of particular interest because their optical and electrical properties can be readily modified. For example, the peak emission frequency of a quantum dot is extremely sensitive to the quantum dot’s radius and composition. This fascinating property gives rise to numerous fabrication techniques.
EARLY FABRICATION METHODS One of the first fabrication methods (that is still being used today) is called colloidal
synthesis. This approach stemmed from Louis Brus’s work at Bell Labs in the late 1970’s. Due to his work, semiconductor quantum dots were grown in the early 1980’s and have since been fabricated into metal and insulator quantum dots. This fabrication method is of great benefit because it is a relatively cheap and simple method; it only requires a reaction flask, a thermometer, two anion precursors and a long-chain solvent. In the case of fabricating semiconductor quantum dots, two common anion precursors are cadmium and selenium. These two precursors can form CdSe quantum dots of varying size that absorb from 410 to 670 nm wavelengths, depending on reaction conditions.
An early lithographic method for creating quantum dots on or near the surface of a semiconductor crystal was used to create a two dimensional structure. This structure was then etched down to a zero-dimensional structure; however, the size of the quantum dot was limited by the resolution of the lithographic steps. The thickness of the semiconductor layer was on the order of nanometers while the other dimensions were as large as a micron. This method was replaced by growing “self-assembled” quantum dots known as the Stranski-Krastanov growth method. This method deposits a semiconductor material with a larger lattice constant (e.g. Germanium) onto a semiconductor material with a smaller lattice constant (e.g. Silicon) causing strained epitaxial growth. This fabrication method has been used to create quantum dot lasers, a device capable of generating single photons and a single photon detector.[2,4]
High dose ion implantation is another method used to fabricate quantum dots. This method is used to create high density encapsulated quantum dots in a host material. These quantum dots (QDs) and host materials range from Si QDs in SiO2 to GaN QDs in Al2O3. Ion implantation produces a supersaturation of an impurity that leads to the formation of QDs encapsulated in the host material after a high temperature annealing process. The electrical and optical properties of the QDs formed by ion implantation depend on the beam current, implant
time, energy, annealing time and temperature. For an example, a simple change in the annealing temperature can either increase or decrease the photoluminescent intensity.
Silicon has been used for decades as an electric material and has only been recently used as an optical material due to its indirect band-gap of 1.12 eV, which is not desirable for an efficient light-emitting device. Due to the numerous fabrication methods of QDs and the well understood fabrication methods used in creating silicon-based microelectronics, a silicon-based integrated optoelectronic circuit was proposed in 1993. This was several years after the first reported visible photo-luminescence in 1990 from silicon QDs by H. Takagi. This proposal has lead to the fabrication of silicon QDs using different methods to produce different optical properties. Some of these fabrication methods include microwave plasma decomposition of SiH4, laser breakdown of SiH4, plasma-enhanced chemical vapor deposition, high frequency discharge, and high dose ion implantation.[5,9,10] In this paper, the formation of silicon QDs by ion implantation will be discussed and compared to that of other fabrication methods resulting in similar optical properties.
FORMATION OF SILICON QUANTUM DOTS BY ION IMPLANTATIION High dose ion implantation is used to create high densities of encapsulated QDs in a wide
range of host materials. This method allows the surface layers of the host material to be doped with an impurity above the solubility limit. However, if the concentration of the impurity exceeds a critical level, precipitation occurs resulting in a reduction of the concentration of the impurity to the solubility limit. As a result, precipitates with a specific size distribution are formed. If the concentration of the impurity does not reach the critical level, the implanted sample is annealed. During this process, a phenomena known as Oswald ripening occurs, causing “coarsening” of the nanoclusters. This action is driven by the minimization of the interfacial energy. According to Gibbs-Thomsons relation, the formation of larger clusters are favored over smaller clusters causing a size distribution throughout the host material. A schematic of the physical processes involved with ion implantation is shown in Figure 1. A high resolution TEM image of Si QDs in SiO2 is shown in Image 1.
Figure 1. Schematic illustration of the formation of
silicon quantum dots with annealing process.
Image 1. High resolution TEM image of Si QDs in SiO2 synthesized
from thermal SiO2 implanted with 50 keV Si ions to a dose of 5x1016/cm2. Annealing was carried out in a vacuum at 1000°C for 40 minutes. 
EFFECTS OF ION IMPLANTATION METHODS ON PHOTOLUMINESCENCE
Silicon QDs that are fabricated with ion-implantation have very different optical properties based on the conditions they were formed. The position and shape of PL spectra depend on the QD’s size and size distribution. The position of PL peaks can be determined by solving the Schrödinger equation for a zero-dimensional quantum structure: (1) 28
mr ihE =Δ
Where the electron state energy above the band gap is ΔE = hυ − Eg with recombination energy hυ, Si band gap Eg = 1.12 eV, effective mass m=0.155*m0, free electron mass m0, QD size r, Planck constant h, and quantum number i. Assuming a Gaussian distribution for the QD size r, the shape of PL spectra can be calculated by using the relation:
With the number of QDs n, mean QD radius r0, coefficient C = h2i2/8m, and ΔE0=C/r02. Thus, Eq. (2) establishes a correlation between the shape of PL spectra and the size r with size distribution σ of QDs.
For an example, photo-luminescence (PL) occurred from a sample of Si implanted in SiO2 with a dose of 3x1016/cm2 (compared to a dose of 6x1017/cm2 at 400 keV) followed by a 1
hour high temperature anneal at 1100ºC with Ar and 4% H2 that was performed by Dr. C.W. White. These experimental conditions resulted in a peak wavelength shift from ~690 nm to ~760 nm (Fig. 2). A weak optical transmission was also observed in the Si QDs implanted in SiO2 after annealing, graphically shown in Figure 3. The absorption edge shifted to a lower energy as the dose and particle size increased. These results are in agreement if the resulting radiation was raised from quantum confined excitations, however interfaces could be partially responsible for the emission. Due to the significantly different energies of optical absorption and PL emissions, it was assumed that the radiation could not have been band-edge emission.
Figure 2. PL arising from Si (400eV) implanted SiO2 Figure 3. Optical transmission measured after annealing at 1100ºC for 1 hour with Ar and 4% H2.  through fused silica samples implanted by Si (400 keV) and annealed at 1100ºC for 1 hour with Ar and H2. Results from the implanted samples were compared with those from un-implanted fused silica.
Hydrogen passivation at different annealing temperatures also affects the PL intensity, the measured luminescence life time, and the number of luminescent QDs. Professor Robert Elliman performed ion implantation on 1.25 μm of thermally grown silicon dioxide layers with 400 keV Si+ ions to a fluence of 2x1017/cm2.The annealing was done at 1000ºC in Ar for 1 hour. Passivation was then achieved by annealing in forming gas (5% H2 in N2) at different temperatures (100-800ºC)